Anionic clays for sunscreen agent safe use photoprotection
Anionic clays for sunscreen agent safe use: Photoprotection,
photostability and prevention of their skin penetration
*, Valeria Ambrogia
, Barbara Bertinia
, Maurizio Riccia
, Loredana Latterinib
, Carlo Rossia
Dipartimento di Chimica e Tecnologia del Farmaco, Universita` degli Studi di Perugia, Perugia, Italy
Dipartimento di Chimica, Universita` degli Studi di Perugia, Perugia, Italy
Received 25 April 2005; accepted in revised form 8 August 2005
Available online 3 October 2005
The use of sunscreen preparations is recently growing and their efﬁcacy and safety must be taken into account since they are applied on the
skin frequently and for many hours. Exposition to sunlight, in fact, can cause sunscreen photodegradation and determine their decrease in UV
protection often with the occurrence of allergic and/or toxic degradation products. A high photostability is hence very important for their
effectiveness and safety.
The aim of this work is to obtain new sunscreen formulations stabilized by intercalating PABA, within the lamellar structures of two kinds
of hydrotalcite. PABA was chosen as model sunscreen because of its high photoinstability and photosensitizing properties that nowadays bar
its utilization. Both intercalated products showed an increased protection range and, in one case, an improved sunscreen photostability.
Sunscreen release from creams containing intercalated or free PABA was evaluated as well. The very low or negligible sunscreen release,
obtained from the intercalated product loaded formulations, resulted in a lack of a close contact between skin and ﬁlter with the consequence
that cutaneous reactions and allergy problems are eliminated.
The use of these materials resulted in a good strategic technological approach in order to increase efﬁcacy and safety of solar products.
q 2005 Elsevier B.V. All rights reserved.
Keywords: Sunscreen agent; para-Aminobenzoic acid; Hydrotalcite; Intercalation; Photoprotection; Photostability
The harmful effects of sunlight, especially the solar UV
radiation, on human skin are well known . Adverse
reactions to the sun UV rays include short-term inﬂamma-
tory responses (erythema, sunburn) and long-term effects
(cutaneous photoageing, immunosuppression and skin
cancers) [1–3], which are increasing throughout the world.
Public hazard awareness to sunlight exposure brought to an
increasingly widespread use of sunscreen agents [1,4,5].
Chemical sunscreens are compounds that absorb UV light
and thereby decrease the amount of the solar radiation
energy reaching the stratum corneum . Most sunscreen
preparations on the market are appropriate only for UV-B
rays, but protection from UV-A rays assumed increasing
importance too since more is known about their adverse
effects on human skin [1,6,7]. The electronically excited
sunscreen molecule can decay through different pathways:
in the form of heat, by ﬂuorescence, phosphorescence,
interaction with neighbouring molecules or by undergoing
photoinduced decompositions [8,9]. The latter reactions
decrease the sunscreen UV-protective capacity during its
use [9–11] and can also produce allergic or toxic
degradation products [4,12]. Therefore a high photostability
is a prerequisite for the effectiveness of sunscreen products.
The p-aminobenzoic acid (PABA) is a UV-B absorber
(200–313 nm)  used as a sunscreen component as early
as the 1920 s and lasted since when dermatologists became
aware that it was a fearly photosensitizer. In fact it tends
to cross-sensitize with other para-molecules  and it is
responsible for adverse cutaneous reactions like irritation,
contact orticaria and allergic and photoallergic dermatitis
European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193
0939-6411/$ - see front matter q 2005 Elsevier B.V. All rights reserved.
* Corresponding author. Dipartimento di Chimica e Tecnologia del
Farmaco, Universita` degli Studi di Perugia, Via del Liceo, 1, Perugia
06123, Italy. Tel.: C39 0755855133; fax: C39 755855163.
E-mail address: email@example.com (L. Perioli).
[15,16]. PABA can decompose to a nitrosamine degradation
product with a known potential carcinogenic effect, so that,
since the late 1980 s, it has been practically withdrawn from
the sunscreen and cosmetic market, and most products
proclaim that they are ‘PABA-free’ .
In the time, photodegradation of chemical sunscreens has
been reduced by providing a protective ﬁlm around the
reacting molecule, by incapsulation in liposomes, micro-
spheres  and in glass beads , incorporation in
nanoparticles  or by complexation with cyclodextrines
. Recently, we demonstrated that intercalation in
inorganic materials as hydrotalcite (HTlc)  could
represent a new strategy to improve sunscreen photo-
stability and to avoid a direct contact with skin.
Hydrotalcites, natural anionic lamellar solids with posi-
tively charged layer balanced by exchangeable anions ,
are rare in nature, but quite easy to prepare in laboratory.
They have the general formula ½MðIIÞ1KxMðIIIÞ1KxðOHÞ2xC
m S where M(II) is a bivalent metal cation, usually
Mg, M(III) is a trivalent metal cation, usually Al, AnK
exchangeable inorganic or organic anion that compensates
the positive charge of the layer and m are the moles of
solvent S, usually water, co-intercalated for mole of
compound . An intercalated anion can be replaced by
another via ion-exchange, with consequent variation of the
interlayer distance . Consequently, the interlayer region
of a lamellar host can be considered a microvessel in which
an anionic molecule may be stored.
The aim of this research is to store the sunscreen in the
interlayer region of a lamellar host and for this purpose we
have chosen HTlc containing magnesium and aluminium
(MgAl–HTlc) or zinc and aluminium (ZnAl–HTlc) cations.
These metals are largely used in cosmetic formulations both
as salts (antiperspirants) and as oxides (ZnO is a physical
sunscreen) [24–30]. PABA has been chosen as sunscreen
model because of its high photoinstability and photosensi-
tizing properties. The expected advantages of sunscreen
intercalation in hydrotalcites are: (i) sunscreen stabilization,
(ii) absorption of ultraviolet lights in both the UV-A region
and the UV-B region and (iii) absence of a close contact
between skin and ﬁlter with the consequent elimination of
allergy problems. With this assumption, a new protection
model has been designed. Thus, the present paper reports
the studies on the intercalation products of PABA into
MgAl–HTlc and ZnAl–HTlc lamellar structures and the
properties of the relative cosmetic formulations.
2. Materials and methods
Well crystallised [Mg0.66Al0.34(OH)2](NO3)0.34$0.4H2O
and [Zn0.66Al0.34 (OH)2](NO3)0.34$0.4H2O was obtained by
co-precipitating, from ‘homogeneous solution’, Mg(II) or
Zn(II) and Al(III) hydroxycarbonate (HTlc–CO3) 
and successive COK
3 ion exchange by titration with
HNO3 0.1 N .
PABA was kindly provided by Farmalabor, Bari (Italy),
polygliceryl-4-isostearate cetyl dimethicone copolyol hexyl
laurate (Abil WE 09) and polygliceryl-3-isostearate (Isolan
GI 34) and cetyl dimethicone (Abil wax 9801) by
Goldschmidt, Cremona (Italy), cyclomethicone (Silicone
DC 245) by Dow Corning, Seneffe (Belgium), Ceresine
(Ceresine wax SP 252) by Rossow Cosme´tiques, Gennevil-
liers (France), Mineral oil was purchased from Carlo Erba,
Milano (Italy). Other chemicals and solvents were of
reagent grade and were used without further puriﬁcation.
2.2.1. Preparation and characterization of intercalation
A carbon dioxide free 0.1 N NaOH water solution
(474 ml) was added to a suspension of 65 g (474 mequiv)
of PABA in degassed water (710 ml) to obtain a sodium salt
solution to which 5 g (19.5 mequiv) of MgAl–HTlc–NO3
were added. The same procedure was followed to intercalate
the sunscreen in ZnAl–HTlc–NO3 by adding a carbon
dioxide free 0.1 N NaOH water solution (569 ml) to a
suspension of 78 g (569 mequiv) of PABA in degassed
water (854 ml). Then 5 g (14.8 mequiv) of ZnAl–HTlc–
NO3 were added. The resulting suspensions were stirred at
60 8C, 140 rpm for 7 days in an orbital incubator. After
cooling, the reaction mixtures were centrifuged at 5000 rpm
for 5 min, washed three times with degassed water, three
times with ethanol and ﬁnally dried at room temperature
over P2O5. The intercalation reactions were performed in an
orbital incubator Gallencamp type INR 2000, Leicester-
shire, UK, and the mixtures were centrifuged with a A.L.C.
centrifuge (Milano, Italy) mod. 4236A.
X-ray powder diffraction patterns (XRDP) were per-
formed with a PW 1710 Philips diffractometer (Lelyweg,
Netherland), using the Ni-ﬁltered Cu Ka radiation. Thermo-
gravimetric analyses were carried out using A Stanton-
Redcroft STA 780 (England) thermoanalyzer at heating rate
of 5 8C minK1
in air ﬂow to determine the weight loss of
water and drug as a function of increasing temperature.
PABA content was also determined by UV analysis at
lmaxZ268.0 nm using a spectrophotometer Jasco-V-520
(Tokyo, Japan) after dissolution of a known amount of
intercalation compound in HCl solution and successive
dilution with phosphate buffer at pH 7.5.
Differential scanning calorimetry analyses (DSC) were
performed using an automatic thermal analyser (Mettler
Toledo DSC821e, Italy). Temperature calibrations were
performed with indium as a standard. Sealed and holed
aluminium pans were used for all the samples and an empty
pan prepared in the same way was used as a reference.
Samples of 3–6 mg were weighted directly into the
aluminium pans and thermal analyses were conducted at
a scanning rate of 10 8C/min from 20 to 500 8C.
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193186
FT-IR spectra were recorded by mean of a Bruker IFS
113 V with source Globar and DTGS rilevator on KBr
tablets and discs of CsI.
Scanning electron microscopy (SEM) photographs were
taken with a Philips SEM 501 (PW 6703) (Holland). Before
observation, the dried samples were sputtered and coated,
for ca. 5 min under an argon atmosphere, with gold–
2.2.2. Intercalated product water-stability
Stability of intercalated products in water  was
performed pouring 100 mg of intercalated products in 50 ml
of deionized water. The suspension was stirred for 2 h at
room temperature and then centrifuged with a 4236A ALC
centrifuge (Milan, Italy) at 4000 rpm for 5 min. The PABA
content in the supernatant was determined by UV absorption
at 268.0 nm.
2.2.3. Preparation of sunscreen creams
The waterproof silicone cream  used for the
sunscreen formulations had the following composition:
1. polygliceryl-4-isostearate cetyl dimethicone copolyol
hexyl laurate (Abil WE-09) 5%, polygliceryl-3-isostea-
rate (Isolan GJ-34) 1%, cyclomethicone (silicone DC-
245) 7.50%, cetyl dimethicone (Abil wax 9801) 3%,
castor oil 0.50%, ceresin (Ceresine wax SP 252) 1%,
mineral oil 2%,
2. HTlc–PABA 10%,
3. deionized water q.b. a 100 g.
The components 1 and 3 were mixed at 80 8C, cooled
down to 60 8C, then the intercalated product (10%) were
added. The resulting PABA content was 2.48% for the
MgAl–HTlc formulation and 2.47% for the ZnAl–HTlc
formulation. Creams containing the same amount of free
PABA (nonintercalated) were prepared as well.
2.2.4. In vitro PABA release from sunscreen creams
The sunscreen release was performed in a dissolution
apparatus for semisolid preparation (Steroglass, Perugia,
Italy) using the Petri disk method . 300 mg of sunscreen
cream were spreaded on the Petri disk (50 mm diameter)
with a spatula to produce an even, uniform surface of
constant dimensions. The paddle rotation speed was kept at
60 rpm and the dissolution medium volume was 100 ml
. The dissolution vessels, closed on the top, were kept in
a thermostatically controlled circulation water bath at 32G
0.5 8C. The dissolution media consisted in deionized water,
phosphate buffer pH 5.5 (Farmacopea Ufﬁciale Italiana XI
Ed.) to simulate the pH skin and NaCl solution (0.4 mg/
100 ml)  in order to simulate the sea water. At
predetermined times, aliquots of 2 ml were removed,
appropriately ﬁltered (13 mm Filter UNIT 0.45 mm NY
PP, Lyda, WI, USA), diluted when necessary and analysed
by UV at lmaxZ268.0 nm in the case of water and saline
solution and at lmaxZ266.4 nm in the case of phosphate
buffer pH 5.5. The removed aliquots were immediately
replaced with the same volume of medium. Tests were made
in triplicate and the results were recorded as an average.
Sunscreen releases from the formulation and from the cream
Fig. 1. X-ray powder diffraction pattern of MgAl–HTlc–NO3 and MgAl–
HTlc–PABA (A); ZnAl–HTlc–NO3 and ZnAl–HTlc–PABA (B).
Fig. 2. Thermogravimetric analysis curves of MgAl–HTlc–PABA and
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193 187
containing not intercalated PABA were performed. For this
reason a silicon cream containing 2.47% of free (not
intercalated) PABA was prepared and the release proﬁles of
all formulations were observed.
2.2.5. Photochemical and photophysical studies
Absorption spectra of the solid samples were recorded by
a spectrophotometer (Perkin–Elmer Lambda 16, England)
equipped with an integration sphere. The spectra recorded
were analysed with the Kubelka–Munk equation in order to
make possible the comparison. The ﬂuorescence spectra and
intensity vs. time for all samples were recorded through a
ﬂuorimeter (Spex Fluorolog 2, USA) using the front face
conﬁguration between the excitation and the emission light.
Spectra were corrected for the instrument response at each
wavelength. The ﬂuorescence intensity vs. irradiation time
was recorded by ﬁxing excitation and emission wavelengths
and by monitoring the emission intensity as function of the
3. Results and discussion
3.1. Preparation and characterisation of intercalation
Synthetic MgAl–HTlc and ZnAl–HTlc in the carbonate
form, prepared as previously described, were not suitable
for PABA intercalation because it is well known  that
carbonate ions are strongly held in the interlayer region and
it is very difﬁcult to replace them with other anions using
simple ion exchange procedures. It is also known that
the monovalent anions as NOK
3  can be more easily
replaced than carbonates; therefore MgAl–HTlc–CO3
Fig. 3. FTIR spectra of free PABA, MgAlHTlc–NO3, ZnAlHTlc–NO3, MgAlHTlc–PABA, ZnAlHTlc–PABA.
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193188
and ZnAl–HTlc–CO3 have been converted into the nitrate
forms . The PABA intercalation has been successfully
obtained by an anion exchange process as described in the
experimental part. The formation of both intercalated
compounds, MgAl–HTlc–PABA and ZnAl–HTlc–PABA,
was conﬁrmed by X-ray powder diffraction spectra
(Fig. 1(A) and (B)) where an increase of the interlayer
distances was observed as a consequence of PABA
intercalation. In the case of MgAl–HTlc–PABA it was
possible to observe the lack at 9.0 A˚ due to MgAl–HTlc–
NO3 and the presence of the peak at 15.5 A˚ relative to the
intercalation of PABA in MgAl–HTlc. Similarly, in the
spectrum of ZnAl–HTlc–PABA the interlayer distance
increased from 9.0 to 15.9 A˚ . In this spectrum, it was
possible to note also a residual peak at 7.6 A˚ due to the
3 ions entrapped between the lamellae.
Fig. 2 shows the thermogravimetric curves of the
intercalation compounds, previously stored in a dessicator
at room temperature and 75% relative humidity. Taking into
account that patterns of the sample heated at 1000 8C
indicate the presence of MgO and MgAl2O4 in the case of
MgAl–HTlc–PABA and ZnO and ZnAl2O4 in the case of
ZnAl–HTlc–PABA, the weight loss curves, as function
of temperature, may be interpreted as follows: from room
temperature to ca. 200 8C samples loose the co-intercalated
water; the great weight losses between 200 and ca. 500 8C is
attributable to the sunscreen decomposition and to the loss
of water due to dehydroxylation of the inorganic layers. The
derived formulas resulted: [Mg0.66Al0.34(OH)2]PABA0.212
(NO3)0.128$1.13H2O (sunscreen content 24.8%) and [Zn0.66-
Al0.34(OH)2]PABA0.258(CO3)0.041$H2O (sunscreen content
24.7%). This means that 248 and 247 mg of PABA were
present, respectively, in 1000 mg of the intercalated
compound. The PABA content was conﬁrmed by UV
analysis after HTlc destruction in acidic medium.
FT-IR spectrum of PABA (Fig. 3) showed two peaks
between 3365 and 3475 cmK1
due to the amine group and a
peak at 1667 cmK1
due to the carboxylic groups. However,
the IR spectrum of MgAl–HTlc–NO3 and ZnAl–HTlc–NO3
showed a broad band between 3200 and 3800 cmK1
, due to
the stretches of hydrogen-bonded hydroxyl group of both
hydroxide layers and interlayer water, and a peak at
, due to the nitrate group. The lack of carboxylic
group absorption and the presence of two peaks at 1401 and
for MgAl–HTlc and at 1397 and 1527 cmK1
ZnAl–HTlc, due to the carboxylate asymmetric and
symmetric stretches relative to the intercalated anions,
were observed as well.
DSC thermogram (Fig. 4) of PABA ((A) and (B))
showed an endothermic peak at ca. 189 8C relative to the
melting point of pure crystalline substance. Thermograms of
HTlc in nitrate form show a large peak around 250 8C
for MgAl–HTlc–NO3 (A) and 380 8C for ZnAl–HTlc–NO3
(B) due to the loss of hydroxyl groups present in HTlc.
In the intercalation compound thermograms, the lack of
the endothermic peak at 189 8C is a conﬁrmation that the
sunscreen intercalation process occurred.
SEM of HTlc–NO3 and HTlc–PABA powders are also
reported (Fig. 5). The images relative to the intercalated
products revealed microcrystals in a nearly hexagonal form
and, in comparison to hydrotalcites in nitrate form, it is
noteworthy to point out that the intercalation process did not
modify either the microcrystal size or the morphology.
3.2. Preparation of sunscreen creams
Sunscreen formulations are generally gels, oils, creams,
milks or sticks; in our case the ideal formulation should
have the following requirements:
1. least presence as possible of water to prevent the ﬁlter
deintercalation from hydrotalcite and consequently to
avoid its contact with the skin;
2. absence of dissolved ions, whose presence could cause
ﬁlter deintercalation from hydrotalcite via ionic
exchange during the cream preparation and storage;
Fig. 4. Differential scanning calorimetry thermograms curves of free
PABA, MgAl–HTlc–NO3 and MgAl–HTlc–PABA (A) and PABA,
ZnAl–HTlc–NO3 and ZnAl–HTlc–PABA (B).
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193 189
3. consistency, spreading, cosmetic pleasantness, water
resistance as requested from a good sunscreen
To fulﬁl these requirements a silicon cream was chosen
because it is not oily and water proof .
3.3. Studies of sunscreen release from formulations
The release of PABA in water was evaluated (Fig. 6(A)).
The PABA is released from cream in a quantity of 20% after
15 min, 43% after 5 h and the release increased up to 81%
after 8 h. The intercalated PABA is released in a much
smaller manner. In fact, the release is less than 5% for the
ﬁrst hour, less than 10% in 5 h and less than 12% in 8 h.
The same release differentiations were observed in
presence of a phosphate buffer (Fig. 6(B)). The release of
PABA, when in free solid state, is 25% in 15 min., around
50% in 6 h and increased up to 67% in 7 h. The PABA
release from both intercalated compounds is around 20%
after 3 h and less than 31% after 8 h.
The nonintercalated PABA release from the cream in sea
water (NaCl salt solution) (Fig. 6(C)) is more than 30% after
15 min and rises to 50% after 2 h, while from the
intercalated formulation is less than 10% after 6 h and less
than 12% in 8 h. These results show that, even after the
contact with sea water, the sunscreen is barely released
while most of it remains entrapped inside the inorganic host
practically avoiding any its skin contact.
3.4. Studies of photophysical and photochemical properties
The absorption spectra of free solid and intercalated
PABA (Fig. 7), are strongly affected by the microenviron-
ment. The spectrum obtained from the free solid PABA
presents a maximun at 320 nm and a shoulder at 415 nm. In
the case of MgAl–HTlc–PABA the main absorption
maximum is centered at 300 nm and the shoulder in the
visible region is more evident than when PABA is in the free
solid state. For the system ZnAl–HTlc–PABA, the
absorption spectrum is markedly red shifted since the
main maximum is at 425 nm and a shoulder at 580 nm was
observed. These effects on the absorption spectra can be due
to speciﬁc interactions between PABA and ZnAl–HTlc
matrix likely because of the formation of complexes
between the nitrogen of the sunscreen and the Zn atoms
present in the inorganic phase [38,39]. The broadening of
the absorption bands observed for ZnAl–HTlc–PABA
leads to an increase of the protection range for the
intercalation compound compared to the free compound.
So, the establishment of these speciﬁc interactions between
the sunscreen and the matrix is wanted to extend its
The emission spectra of samples under investigation are
recorded. The spectrum of free solid PABA shows a broad
band centered at 420 nm while the spectra obtained from the
intercalated samples show a main maximum at 345 nm and
a broad band between 400 and 550 nm. It is likely that
the band centered at 345 nm is due to the chromophore
Fig. 5. Scanning electron micrography of HTlc–NO3 and intercalation compounds.
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193190
externally adsorbed on the hydrotalcite, while the red-band
is the contribution of the intercalated molecules, as already
observed for other dye–hydrotalcite composite . It is
noteworthy to point out that excitation of the inorganic
matrix alone did not lead to a detectable emission (data not
The high sensitivity of the emission measurements was
used to test and compare the photostability of the samples
under investigation. In particular, emission spectra of
all samples, were recorded in the same experimental
conditions, before and after irradiation at 297 nm for 2 h.
No changes in the spectral shape were observed. However,
an emission intensity decrease was detected in the not
normalized spectra (see below) indicating the occurrence of
photodegradation processes leading to products that do not
emit in the used experimental conditions. Since the
photoproducts did not interfere with the emission properties
of PABA-compounds, the photostability analysis was
pushed further considering that all samples absorb a similar
amount of the excitation light (297 nm, Fig. 7). In order to
have kinetic information on the chromophore concentration
change in the irradiated area, the decrease of emission
intensity was followed as function of irradiation time for all
compounds under investigation. In particular, the emission
traces (Fig. 8) were recorded during the irradiation at
297 nm by collecting the emission at the maximum for each
Fig. 6. Release of PABA from creams containing free PABA, MgAl–
HTlc–PABA and ZnAl–HTlc–PABA in water (A), in phosphate buffer at
pH 5.5 (B), in sea water (C).
Fig. 7. Absorption spectra of MgAl–HTlc–PABA (1), free PABA (2) and
Fig. 8. Fluorescence decay of free PABA, ZnAl–HTlc–PABA and MgAl–
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193 191
sample. The traces shown in Fig. 8 indicated that the
emission of free PABA and of MgAl–HTlc–PABA
decreases with a similar behavior to reach 78% of the
initial value during the irradiation. In the case of ZnAl–
HTlc–PABA, the emission decreases slower and in 2 h only
10% reduction was observed. Thus, the ZnAl–HTlc matrix
well improves the photochemical stability of PABA,
protecting the molecule from photodegradation reactions.
The comparison of the data obtained from the two
intercalation compounds suggests that the higher stability
of ZnAl–HTlc–PABA system is not only due to a physical
screen (similar for both matrices), but also to a chemical
protection of the photoactive chromophore.
The spectroﬂuorimetric investigation was then carried
out on the samples obtained by dispersing the intercalation
compounds in the siliconic cream. The absorption and
emission spectra of these samples were recorded to
investigate the occurrence of speciﬁc interactions among
the intercalation compounds and the formulation com-
ponents. The absorption spectra of creams loaded with the
intercalated sunscreen presented a shape similar to those of
not formulated intercalation compounds (Fig. 7) but they
have an intensity 2–3 fold higher. This effect is due to the
contribution of cream ingredients to the screening properties
of the intercalation compounds, leading to a higher
protection factor. The emission spectra of the intercalation
compounds in the cream formulation are similar to those of
the intercalated compounds with the same maxima. This
observation indicates that the energy of the emitting state
does not change when HTlc–PABA is dispersed in creams
probably because the interactions between the chromophore
and the cream components are negligible.
To evaluate the photostability of the creams with the
intercalated solar screen, their emission signal was recorded
as function of the irradiation time (Fig. 9). Both creams
showed a reasonable photostability since, after 1 h of
irradiation, only a reduction of ca. 20% of the signal,
attributable to degradation of the chromophore, was
observed. In particular, as already noticed for the
intercalation compounds, ZnAlHTlc–PABA formulation
appeared slightly more stable as well.
The aim of the present research was to store a model
compound sunscreen, such as PABA, whose high instability
and photoreactivity is well known, in the interlayer region of
the lamellar host to study the protection and the sunscreen
modiﬁed release offered by HTlc lamellar structures.
It was thus observed that
1. The intercalation process leads to nanocomposite
materials that extend the solar screen protection range.
2. In the case of the ZnAlHTlc–PABA system, a high
photostability is observed due probably to the establish-
ment of speciﬁc interactions between the matrix and the
3. The intercalation compound, when dispersed in the
formulation, maintained its spectral properties (absorp-
tion and emission) suggesting that the interaction among
the solar ﬁlter and the components of the creams are
4. The photostability of the intercalated PABA creams was
5. The release of PABA from creams containing HTlc–
PABA was negligible (in water and sea water) or very
low (in phosphate buffer) and always much lower than
from creams containing not intercalated PABA.
It is possible thus, to conclude that the intercalation of
PABA into hydrotalcite proved to be very useful to enhance
its sunscreen properties in terms of protection range and
photostability. In fact the use of these new systems
represents a promising, good, efﬁcient way to protect
other chemical ﬁlters having similar photoinstability.
Moreover, since these novel formulations allow a very
low sunscreen release from the formulations, they avoid a
close contact between skin and ﬁlter and hence prevent any
cutaneous reactions and allergy problems that may occur.
The authors are very much grateful to Prof. Umberto
Costantino and Gian Gaetano Aloisi, from the Department
of Chemistry of the University of Perugia, for their valuable
suggestions. This work was supported by MURST (Coﬁn
Fig. 9. Fluorescence decay of formulations containing 10% intercalation
products MgAl–HTlc–PABA and ZnAl–HTlc–PABA.
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193192
 National Institute of Health, National Institute of Health Consensus
Statement Online Sunlight, Ultraviolet Radiat. Skin. 7 (1989) 1–29.
 M.A. Pathak, Ultraviolet radiation and the development of non-
melanoma and melanoma skin cancer: clinical and experimental
evidence, Skin Pharmacol. 4 (1991) 85–94.
 A. Ziegler, A.S. Jonason, D.J. Leffell, J.A. Simon, H.W. Sharma,
J. Kimmelman, L. Remington, T. Jacks, D.E. Brash, Sunburn and p53
in the onset of skin cancer, Nature 372 (1994) 773–776.
 S.H. Dromgoole, H.I. Maibach, Sunscreening agent intolerance:
contact and photocontact sensitization and contact urticaria, J. Am.
Acad. Dermatol. 22 (1990) 1068–1078.
 A. Schrader, J. Jakupovic, W. Baltes, Photochemical studies on trans-
3-methylbutyl 4-methoxycinnamate, J. Soc. Cosmet. Chem. 45 (1994)
 W. Schwack, T. Rudolph, Photochemistry of dibenzoylmethane UVA
ﬁlters, J. Photochem. Photobiol. B: Biol. 28 (1995) 229–234.
 J. Lehmann, D. Pollet, S. Peker, V. Steinkraus, U. Hoppe, Kinetics of
DNA strand breaks and protection by antioxidants in UVA or UVB
irradiated HaCaT keratinocytes using the single cell gel electrophor-
esis assay, Mutat. Res. 407 (2) (1998) 97–108.
 J.K. Broadbent, B.S. Martincigh, M.W. Raynor, L.F. Salter,
R. Moulder, P. Sjoberg, K.E. Markides, Capillary supercritical ﬂuid
chromatography combined with atmospheric pressure chemical
ionisation mass spectrometry for the investigation of product
formation in the sunscreen absorber 2-ethylhexyl-p-methoxycinna-
mate, J. Chromatogr. A 732 (1996) 101–110.
 R. Stokes, B. Diffey, In vitro assessment of sunscreen photostability:
the effect of radiation source, sunscreen application thickness and
substrate, Int. J. Cosmet. Sci. 21 (1999) 341–351.
 G. Berset, H. Gonzenbach, R. Christ, R. Martin, A. Deﬂandre,
R. Mascotto, J.D. Jolley, W. Lowell, R. Pelzer, T. Stiehm, Proposed
protocol for the determination of photostability. Part I: cosmetic UV
ﬁlters, Int. J. Cosmet. Sci. 18 (1996) 167–177.
 N. Tarras-Wahlberg, G. Stenhagen, O. LarkO¨ , A. Rose´n,
A.M. Wennberg, O. WennerstrO¨ m, Changes in ultraviolet absorption
of sunscreens after ultraviolet irradiation, J. Invest. Dermatol. 113
 A. Deﬂandre, G. Lang, Photostability assessment of sunscreens.
Benzylidene camphor and dibenzoylmethane derivatives, Int.
J. Cosmet. Sci. 10 (1988) 53–62.
 M. Ambrosio, I prodotti solari, Cosmesi Dermatologica 41 (1992)
 B. Macie, L. Macie, The PABA story, Australas J. Dermatol 40 (1999)
 T. Cantrell, N. Jussel, S. Morris, Sun damage and skin protection,
Pharmaceutics 425 (2002) 1–8.
 A. Darvay, I.R. White, R.J. Rycroft, A.B. Jones, J.L.M. Hawk,
J.P. McFadden, Photoallergic contact dermatitis is uncommon, Br.
J. Dermatol. 45 (2001) 597–601.
 H.H. Tonnesen, Formulation and stability testing of photolabile, Int.
J. Pharm. 225 (2001) 1–14.
 Merck KGaA- Technology, Darmstadt (Germany). Sunscreens in
glass beads, 2002 http://pb.merck.de/servlet/PB/menu/
 S.A. Wissing, R.H. Mu¨ller, Solid lipid nanoparticles as carrier for
sunscreens: in vitro release and in vivo skin penetration, J. Control.
Release 81 (2002) 225–233.
 S. Scalia, A. Molinari, A. Casolari, A. Maldotti, Complexation of the
sunscreen agent, phenylbenzimidazole sulphonic acid with cyclodes-
trins: effect on stability and photo-induced free radical formation, Eur,
J. Pharm. Sci. 22 (2004) 241–249.
 C. Rossi, A. Schoubben, M. Ricci, L. Perioli, V. Ambrogi, L.
Latterini., G.G. Aloisi, A. Rossi, Intercalation of the radical
scavenger ferulic acid in hydrotalcite-like anionic clays, Int. J.
Pharm. 295 (2005) 47–55.
 F. Cavani, F. Triﬁro`, A. Vaccari, Hydrotalcite-type anionic
clays: preparation, properties and applications, Catal. Today 11
 V. Ambrogi, G. Fardella, G. Grandolini, L. Perioli, M.C. Tiralti,
Intercalation compounds of hydrotalcite-like anionic clays with anti-
inﬂammatory agents, II: uptake of diclofenac for a controlled release
formulation, AAPS Pharm, Sci. Tech. 3 (2002) 1–8.
 R. Machorro, J.M. Siqueiros, S. Wang, Optical properties of Mg, from
UV to IR, using ellipsometry and reﬂectometry, Thin Solid Films 269
 T. Yutaka, S. Orie, Ultraviolet absorber and composition containing
same, Jpn. Patent 11166173 (1999).
 O. Mamoru, M. Hisahiro, Resin particles coating with alumina or
zirconia for sunscreens, Jpn. Patent 2049717 (1990).
 S. Chodorowski, F.X. Quinn, C. Sanchez, Cosmetic sunscreens
comprising an organic UV-A ﬁlter and method for displacing the
maximum absorption wavelength, PCT Patent 2001024768 (2001).
 M. Wada, H. Fukui, T. Kanamaru, Phototoxicity-preventing
compositions consisting of metal oxide-doped photocatalyst powders,
Jpn. Patent 11279019 (1999).
 S. Miyata, Ultraviolet light absorber and its use. EP Patent 1136060
 H.N. Graham, Sunscreen compositions containing sunscreening
agents and zinc oxide, PCT Patent 9852525 (1998).
 U. Costantino, F. Marmottini, M. Nocchetti, R. Vivani, New synthetic
route to hydrotalcite-like compounds, Characterisation and properties
of the obtained materials, Eur. J. Inorg. Chem. (1998) 1439–1446.
 D.L. Bish, Anion-exchange in takovite: applications to other
hydroxide minerals, Bull. Mineral. 103 (1980) 170–175.
 S. Carr, K. Franklin, C. Nunn, J. Pasternak, I.R. Scott, Sunscreen
agents US Patent 5474762 (1995).
 Waterproof sunscreens. Cosmetics & Toiletries, It. Ed, 2 (1997) 58.
 B.J. Poulsen, E. Young, V. Coquilla, M. Katz, Effect of topical vehicle
composition on in vitro release of ﬂuocinolone acetonide and its
acetate ester, J. Pharm. Sci. 57 (1968) 928–933.
 Z.T. Chowhan, R. Pritchard, Release of corticoids from oleaginous
ointment bases containing drug in suspension, J. Pharm. Sci. 64
 M. Fresno, J. Contreras, M.M. Jime´nez Soriano, E. Selles Flores,
Prodotti solari: formulazioni, Cosmet. News 138 (2001) 163–165.
 J.S. Yang, Y.D. Lin, Y.H. Lin, F.L. Liao, Zn(II)- Induced ground-state
p-deconiugation and excited state electron transfer in N,N-Bis(2-
pyridyl)amino-substituted arenas, J. Org. Chem. 69 (2004) 3517–
 S. Wang, Luminescence and electroluminescence of Au(III), B(III),
Be(II) and Zn(II) complexes with nitrogen donors, Coord, Chem. Rev.
215 (2001) 79–98.
 L. Latterini, F. Elisei, G.G. Aloisi, U. Costantino, M. Nocchetti,
Space-resolved ﬂuorescence properties of phenolphalein-hydrotalcite
compounds, Phys.Chem. Chem. Phys. 4 (2002) 2792–2798.
L. Perioli et al. / European Journal of Pharmaceutics and Biopharmaceutics 62 (2006) 185–193 193